Synthesis and Chirality Control of Bulk Crystals and Nanocrystals: From a Right-Handed Nonpolar Chain to a Left-Handed Polar Chain
Yan-Yan Yin; Yan-Li Zhao; Jian-Gong Ma; Xiao-Chang Cao; Peng Cheng; Inorganic Chemistry 52 (2013) 3738–3743; doi:10.1021/ic302711b

data_4334334
_publ_section_title
;
 Synthesis and Chirality Control of Bulk Crystals and Nanocrystals: From a
 Right-Handed Nonpolar Chain to a Left-Handed Polar Chain
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              3738
_journal_page_last               3743
_journal_paper_doi               10.1021/ic302711b
_journal_volume                  52
_journal_year                    2013
_chemical_absolute_configuration ad
_chemical_formula_sum            'C5 H11 Cu N O7 S'
_chemical_formula_weight         292.75
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           4
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 102.08(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   5.1721(10)
_cell_length_b                   9.773(2)
_cell_length_c                   9.867(2)
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25.01
_cell_measurement_theta_min      2.97
_cell_volume                     487.70(17)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0581
_diffrn_reflns_av_sigmaI/netI    0.1163
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -4
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            1811
_diffrn_reflns_theta_full        25.01
_diffrn_reflns_theta_max         25.01
_diffrn_reflns_theta_min         2.97
_exptl_absorpt_coefficient_mu    2.470
_exptl_absorpt_correction_T_max  0.6379
_exptl_absorpt_correction_T_min  0.4382
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            blue
_exptl_crystal_density_diffrn    1.993
_exptl_crystal_description       prism
_exptl_crystal_F_000             298
_exptl_crystal_size_max          0.40
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.20
_refine_diff_density_max         2.279
_refine_diff_density_min         -1.270
_refine_diff_density_rms         0.261
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.08(6)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.018
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     154
_refine_ls_number_reflns         1434
_refine_ls_number_restraints     12
_refine_ls_restrained_S_all      1.013
_refine_ls_R_factor_all          0.1108
_refine_ls_R_factor_gt           0.0980
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.1568P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2289
_refine_ls_wR_factor_ref         0.2389
_reflns_number_gt                1155
_reflns_number_total             1434
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic302711b_si_001_2.cif
_cod_data_source_block           b
_cod_original_cell_volume        487.73(17)
_cod_database_code               4334334